The structure described by V2(OF)3 crystallizes in the triclinic P1 space group. There are six inequivalent V sites. In the first V site, V(1) is bonded to one O(4), one O(7), one O(9), one F(3), one F(5), and one F(8) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 21-37°. In the second V site, V(2) is bonded to one O(1), one O(3), one O(8), one F(4), one F(7), and one F(9) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 17-40°. In the third V site, V(3) is bonded to one O(1), one O(3), one O(6), one F(1), one F(2), and one F(9) atom to form corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 17-40°. In the fourth V site, V(4) is bonded to one O(4), one O(6), one O(9), one F(1), one F(2), and one F(5) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 22-34°. In the fifth V site, V(5) is bonded to one O(2), one O(5), one O(7), one F(3), one F(6), and one F(8) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 16-37°. In the sixth V site, V(6) is bonded to one O(2), one O(5), one O(8), one F(4), one F(6), and one F(7) atom to form corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 16-37°. There are nine inequivalent O sites. In the first O site, O(1) is bonded in a bent 150 degrees geometry to one V(2) and one V(3) atom. In the second O site, O(2) is bonded in a bent 150 degrees geometry to one V(5) and one V(6) atom. In the third O site, O(3) is bonded in a linear geometry to one V(2) and one V(3) atom. In the fourth O site, O(4) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. In the fifth O site, O(5) is bonded in a bent 150 degrees geometry to one V(5) and one V(6) atom. In the sixth O site, O(6) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the seventh O site, O(7) is bonded in a distorted bent 150 degrees geometry to one V(1) and one V(5) atom. In the eighth O site, O(8) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the ninth O site, O(9) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. There are nine inequivalent F sites. In the first F site, F(1) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the second F site, F(2) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the third F site, F(3) is bonded in a bent 150 degrees geometry to one V(1) and one V(5) atom. In the fourth F site, F(4) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the fifth F site, F(5) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. In the sixth F site, F(6) is bonded in a linear geometry to one V(5) and one V(6) atom. In the seventh F site, F(7) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the eighth F site, F(8) is bonded in a bent 150 degrees geometry to one V(1) and one V(5) atom. In the ninth F site, F(9) is bonded in a bent 150 degrees geometry to one V(2) and one V(3) atom. is represented by the CIF file [CIF]
data_V2(OF)3
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.173
_cell_length_b   5.227
_cell_length_c   13.238
_cell_angle_alpha   91.153
_cell_angle_beta   90.232
_cell_angle_gamma   119.530
_symmetry_Int_Tables_number   1
_cell_volume   311.388
_cell_formula_units_Z   3
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  V  V0  1  0.995  0.973  0.487  1.0
  V  V1  1  0.953  0.982  0.999  1.0
  V  V2  1  0.641  0.325  0.158  1.0
  V  V3  1  0.376  0.675  0.329  1.0
  V  V4  1  0.716  0.347  0.665  1.0
  V  V5  1  0.333  0.640  0.825  1.0
  O  O6  1  0.349  0.250  0.083  1.0
  O  O7  1  0.977  0.573  0.752  1.0
  O  O8  1  0.776  0.091  0.082  1.0
  O  O9  1  0.084  0.760  0.417  1.0
  O  O10  1  0.411  0.428  0.750  1.0
  O  O11  1  0.579  0.582  0.254  1.0
  O  O12  1  0.910  0.253  0.588  1.0
  O  O13  1  0.671  0.762  0.919  1.0
  O  O14  1  0.662  0.908  0.419  1.0
  F  F15  1  0.998  0.421  0.254  1.0
  F  F16  1  0.408  0.998  0.251  1.0
  F  F17  1  0.325  0.086  0.587  1.0
  F  F18  1  0.074  0.334  0.920  1.0
  F  F19  1  0.257  0.339  0.421  1.0
  F  F20  1  0.580  0.009  0.751  1.0
  F  F21  1  0.246  0.924  0.920  1.0
  F  F22  1  0.741  0.666  0.585  1.0
  F  F23  1  0.936  0.675  0.083  1.0
[/CIF]
.
The structure described by V2(OF)3 crystallizes in the triclinic P1 space group. There are six inequivalent V sites. In the first V site, V(1) is bonded to one O(4), one O(7), one O(9), one F(3), one F(5), and one F(8) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 21-37°. In the second V site, V(2) is bonded to one O(1), one O(3), one O(8), one F(4), one F(7), and one F(9) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 17-40°. In the third V site, V(3) is bonded to one O(1), one O(3), one O(6), one F(1), one F(2), and one F(9) atom to form corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 17-40°. In the fourth V site, V(4) is bonded to one O(4), one O(6), one O(9), one F(1), one F(2), and one F(5) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 22-34°. In the fifth V site, V(5) is bonded to one O(2), one O(5), one O(7), one F(3), one F(6), and one F(8) atom to form distorted corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 16-37°. In the sixth V site, V(6) is bonded to one O(2), one O(5), one O(8), one F(4), one F(6), and one F(7) atom to form corner-sharing VO3F3 octahedra. The corner-sharing octahedral tilt angles range from 16-37°. There are nine inequivalent O sites. In the first O site, O(1) is bonded in a bent 150 degrees geometry to one V(2) and one V(3) atom. In the second O site, O(2) is bonded in a bent 150 degrees geometry to one V(5) and one V(6) atom. In the third O site, O(3) is bonded in a linear geometry to one V(2) and one V(3) atom. In the fourth O site, O(4) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. In the fifth O site, O(5) is bonded in a bent 150 degrees geometry to one V(5) and one V(6) atom. In the sixth O site, O(6) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the seventh O site, O(7) is bonded in a distorted bent 150 degrees geometry to one V(1) and one V(5) atom. In the eighth O site, O(8) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the ninth O site, O(9) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. There are nine inequivalent F sites. In the first F site, F(1) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the second F site, F(2) is bonded in a bent 150 degrees geometry to one V(3) and one V(4) atom. In the third F site, F(3) is bonded in a bent 150 degrees geometry to one V(1) and one V(5) atom. In the fourth F site, F(4) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the fifth F site, F(5) is bonded in a bent 150 degrees geometry to one V(1) and one V(4) atom. In the sixth F site, F(6) is bonded in a linear geometry to one V(5) and one V(6) atom. In the seventh F site, F(7) is bonded in a bent 150 degrees geometry to one V(2) and one V(6) atom. In the eighth F site, F(8) is bonded in a bent 150 degrees geometry to one V(1) and one V(5) atom. In the ninth F site, F(9) is bonded in a bent 150 degrees geometry to one V(2) and one V(3) atom. is represented by the CIF file [CIF]
data_V2(OF)3
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.173
_cell_length_b   5.227
_cell_length_c   13.238
_cell_angle_alpha   91.153
_cell_angle_beta   90.232
_cell_angle_gamma   119.530
_symmetry_Int_Tables_number   1
_cell_volume   311.388
_cell_formula_units_Z   3
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  V  V0  1  0.995  0.973  0.487  1.0
  V  V1  1  0.953  0.982  0.999  1.0
  V  V2  1  0.641  0.325  0.158  1.0
  V  V3  1  0.376  0.675  0.329  1.0
  V  V4  1  0.716  0.347  0.665  1.0
  V  V5  1  0.333  0.640  0.825  1.0
  O  O6  1  0.349  0.250  0.083  1.0
  O  O7  1  0.977  0.573  0.752  1.0
  O  O8  1  0.776  0.091  0.082  1.0
  O  O9  1  0.084  0.760  0.417  1.0
  O  O10  1  0.411  0.428  0.750  1.0
  O  O11  1  0.579  0.582  0.254  1.0
  O  O12  1  0.910  0.253  0.588  1.0
  O  O13  1  0.671  0.762  0.919  1.0
  O  O14  1  0.662  0.908  0.419  1.0
  F  F15  1  0.998  0.421  0.254  1.0
  F  F16  1  0.408  0.998  0.251  1.0
  F  F17  1  0.325  0.086  0.587  1.0
  F  F18  1  0.074  0.334  0.920  1.0
  F  F19  1  0.257  0.339  0.421  1.0
  F  F20  1  0.580  0.009  0.751  1.0
  F  F21  1  0.246  0.924  0.920  1.0
  F  F22  1  0.741  0.666  0.585  1.0
  F  F23  1  0.936  0.675  0.083  1.0
[/CIF]
.